Passive Damping Characteristics of Carbon Epoxy Composite Plates


 Stephen Turner
 2 years ago
 Views:
Transcription
1 Journal of aterials Science and Engineering A 6 (12) (2016) doi: / / D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty of echanical Engineering, JT University Kakinada, Kakinada , India Abstract: Vibration damping is an important phenomenon in the field of engineering design while predicting the dynamic analysis of the most of the structures. It is one of the typical dynamic responses of structural members, which allows the members fail due to larger amplitudes. Composite materials are replacing conventional structural materials due to attractive, superior mechanical properties such as high strength to weight ratio, high modulus, high corrosion resistance and good fatigue resistance. Composite materials possess high degree of material damping compared with conventional materials. One of the advanced technique employed to safe guard against the severe intensity of vibrations by controlling the dynamics of the structures is the provision of enhancing energy dissipation by the design of a constrain layer. When a constrain layer is made of a non actuating stiff layer of material introduced in the structure, say a viscoelastic material called a PCLD (Passive constrained layer damping). In the present work, an analytical solution for damping of a FRP (Fiber reinforced polymer) plates with a single or double interleaved viscoelastic layers in is obtained. Ritz method is employed to predict the damping nature of the plate under several boundary conditions. Specific damping capacity and a loss factor are deduced from the method of energy formulation for viscoelastic layers interleaved in laminated fiber reinforced plate. The loss factor of constrain layered plate is calculated as a function of fiber orientation in its orthotropic layers. An isotropic constrain layers are configured at midplane, symmetric, asymmetric and outer positions across the thickness of the plate. A parametric study also carried out to observe the effect of position of a constant thickness viscoelastic layer on the damping characteristics of passively constrain orthotropic plate. Key words: Thin plate theory, specific damping capacity, loss factor and viscoelastic materials. omenclature U: Energy dissipated U: aximum strain energy A mn : Fourier Coefficient of deflection R: Aspect ratio e 0 : Viscoelastic layer of thickness a: Length of the plate b: Width of the plate e: Thickness of the orthotropic lamina iq pq : Reduced stiffness constants d 1 : Up Distance of VEL from laminate idplane d 2 : Down of VEL from laminate idplane w 0 : Transverse displacement A ij : Series Coefficient C minj : Product of integrals I and J D pq : Time E: Young s modulus ort : Bending oment in y direction D pq * Corresponding author: Dileep Kumar K, assistant professor, research field: damping of composite structure. f pq (θ): Orientation function Greek Letters υ : Poisons ratio of VE ψ x : Specific Damping Coefficient λ m: Boundary values of the plate in xdirection γ m: Boundary values of the plate in ydirection η: Loss factor α: Longitudinal modulus α 1 : A constant for VE position Up Distance α 2 : A constant for VE position down Distance 1. Introduction owadays an increased demand for the control of acoustics and vibration in structures had enforced the designers to take damping into account even from the preliminary design phase. A designer always looks for a material which shows superior or optimum properties under given operating environment. It is very difficult task to search for an optimal material for
2 36 Passive Damping Characteristics of Carbon Epoxy Composite Plates every new design. In such cases a composite material will be the best practical solution owing to reason that its properties can be tailored according to desired degree of magnitude by providing geometric and material symmetry conditions. The advantages of composites can be made utilized by the rational choice of stacking sequence. In many aerospace, commercial and automotive components, sports and structures composites have been successfully used. Advanced composite materials not only have high stiffness but also have greater damping capacity compared to metals. For example, in a FRP composite, the damping is enhanced due to the internal friction among the constituents and interfacial slip at the fibermatrix interfaces, where as the fiber contributes to the stiffness. However, the damping capacity of the composite laminates can be increased many fold by incorporating viscoelastic layers between the laminae of the host composite. In this hybrid approach, the dominant mechanism of damping is the shear induced between the damping layer and the constraining layers. The tradeoffs in using damping layers are a slight reduction in stiffness and a small increase in the weight of the composite system. The desirable damping characteristics and design flexibility make the viscoelastic materials to be embedded as an important isotropic constituent layer in the composites. Adams R D [1] consider the basic elasticity relationships for unidirectional composites, together with the AdamsBacon damping criterion, are utilised for prediction of moduli and flexural damping of anisotropic CFRP (Carbon fiber reinforced polymer) and GRP beams with respect to fibre orientation. Billups E K [2] works on several twodimensional theories for investigating the SDC (Specific damping capacity) of composite materials and theories are compared with those of Adams and Bacon, Adams and aheri, i and Adams [3] and Saravanos and Chamis. o interlaminar effects are considered. The analysis considers the variations of Young s modulus and damping of viscoelastic layers with the frequency. Finally, the article presents the effects of Young s modulus and the damping of a viscoelastic layer interleaved in the middle plane of unidirectional laminate by Jeanarie Berthelot [4]. The optimal layup design problem, a layer wise optimization (LO) method is applied to the orthotropic plates comprised of two different laminates, and an optimal fiber angles are determined to obtain the maximum loss factor in the first mode by Jinqiang Li [5]. Jeanarie Berthelot [6] also predicted various damping parameters and are investigated using cantilever beam test specimens using an impulse hammer technique. Damping modeling is developed by a finite element analysis which evaluated the different energies dissipated in the material as a function of fiber directions of the layers is the work of i, R. G. and Adams, R. D [7]. Advanced FRP composites are prime candidates for several interesting applications where damping is a key parameter. Improvement of vibration damping characteristics of such materials makes them qualify even more attractive applications. Since most of composite structural elements in military, automotive and space applications are subject to severe dynamic loads an additional vibration control becomes necessary. This can be achieved by using different damping treatments. High degree of damping in a structure can often improve performance in a dynamic load environment. Various methods for predicting damping in a structure are proposed, the Ritz method is the most efficient method. In composite base structures, several factors influence its structural vibration response. For example, the constituents, the fiber orientation and stacking sequence in the host structure, and the position from midplane, amount and type of treatment of embedded layer, influence the response strongly. The effect of some of such parameters is presented here using Ritz method.
3 Passive Damping Characteristics of Carbon Epoxy Composite Plates odeling of FRP Plate Using Ritz ethod Passive damping has been recognized as an important mechanism for controlling the elastodynamic performance of flexible structures. The arrangement of different layers in a PCLD plate is shown in Fig. 1. Among various passive damping techniques, it is known that the material damping can effectively improves the capabilities for suppressing vibration, sound, fatigue endurance and impact resistance, and can be easily implemented as viscoelastic layers in the laminated plate structures. The goal of an effective damping treatment is to add the viscoelastic material in such a way and in such location so as to ensure that the greatest possible cyclic deformation of the damping materials will occur as the structure vibrates in the modes of interest, to dissipate as much vibrational energy during each cycle as possible. This requires an understanding of the dynamic behavior of the structure or machine and an understanding of the deformation of the viscoelastic material which occurs during vibration of the structure, and by no means least, an understanding of the complex modulus properties of the candidate damping materials in order that a proper treatment can be developed. Two types of laminates with viscoelastic layers were considered. Laminates with a single viscoelastic layer of thickness e 0 interleaved in the middle plane of laminates (Fig. 2) and laminates with two viscoelastic layers of thickness e 0 interleaved away from the middle plane (Fig. 3). The layers of the initial laminates are constituted of unidirectional or orthotropic materials with material directions making an angle θ with the x direction oriented along the length of plates under consideration. The total thickness of the unidirectional or orthotropic layers is e and the interlaminar layers are assumed to have an isotropic behavior orthotropic material of thickness e in which a single viscoelastic layer of thickness e 0 is interleaved (Fig. 2). aterial directions make an angle θ with the plate directions. According to the results established in Berthelot, the total strain energy stored in the laminate with the viscoelastic layers can be expressed as U = U 11 +2U 12 + U 22 + U 66 U pq = U ort v (1) pq + U pq pq = 11,12,22,66 The energies U 11 and U 22 are the strain energies stored in tensioncompression in the material directions, U 12 is the coupling energy induced by the Poisson s effect, and U 66 is the strain energy stored in inplane shear. The energy is separated as the strain ort energy U pq stored in the orthotropic layer and the v strain energy U pq stored in the viscoelastic layer. Applying the results obtained by Berthelot and Sefrani et al and Berthelot, the energy stored in the orthotropic layers 1 and 3 (Fig. 2) can be written as U ort pq = U 1 pq + U 3 pq = 1 A e 2Ra mna 2 ij f pq (θ)q 3 m=1 n=1 i=1 j=1 pq e0e3 e0e3 (2) where, a is the length and R the lengthtowidth ratio of the plate, U 1 3 pq and U pq are the strain energies stored in layers 1 and 3, are the reduced stiffness constants of the materials, and f pq (θ)are functions of the material directions obtained by Berthelot et. al. In the same way, the strain energy stored in the viscoelastic layer is given by 2.1 Interlaminar Viscoelastic Layer The laminate is constituted of a unidirectional or Fig. 1 Laminate with viscoelastic layer.
4 38 Passive Damping Characteristics of Carbon Epoxy Composite Plates will be simply noted. The damping of the viscoelastic layer is related essentially to the Young s modulus and it can be written as ψ v 11 ψ v 22 ψ v 66 ψ v ; ψ v 12 = 0 (7) ext, the damping of laminated plate with a single viscoelastic layer is evaluated by ψ x = ΔU U (8a) Fig. 2 Laminate with a single viscoelastic layer. Finally the loss factor is obtained as follows U v pq 2 = U pq v e 0 3 = 1 2Ra 2 A mna ij f v pq (θ v )iq pq 12 m=1 n=1 i=1 j=1 (3) v where, the reduced stiffness constants iq pq are expressed as E (1 υ 2 ) iq v E pq = (1 υ 2 ) E (1 υ 2 ) E (1 υ 2 ) E 2(1 + υ) (4) Introducing the Young s modulus E and the Poisson s ratio υ of the viscoelastic layer. This layer being considered as isotropic, the results are independent of the direction. Thus, the function f v pq (θ v ) can be deduced by considering an orientation equal to zero, which leads to f v 11 (θ v ) = C 2200 minj ; f v 12 (θ v ) = C 2002 minj R 2 ; f v 22 (θ v ) = C 0022 minj R 4 ; f v 66 (θ v ) = 4C 1111 minj R 2 ; (5) The energy dissipated by viscous damping is then expressed by n U = (ψ ort pq U ort pq + ψ v pq U v pq ) pq (6) Introducing the specific damping coefficients of the orthotropic material considered and the coefficients of the viscoelastic layer. The damping coefficients are the inplane damping coefficients of the orthotropic layer considered in Berthelot and Sefrani et al. They η = ψ x 2π 2.2 Two Interlaminar Viscoelastic Layers (8b) This subsection considers the case of a unidirectional or orthotropic material of thickness e in which two viscoelastic layers of thicknesses e 0 are interleaved in the initial material (Fig. 3). To obtain a general analysis, the viscoelastic layers are considered to be interleaved at distances d 1 and d 2 from the middle plane, respectively. These distances will be expressed as e d 1 = α 1 2, d e 2 = α 2 (9) 2 As previously mentioned, the strain energy stored in the laminate with the two interleaved viscoelastic ort layers can be expressed by Eqn.1 where U pq is the v strain energy stored in the orthotropic layers and U pq is the strain energy stored in the two viscoelastic layers. The strain energy stored in the orthotropic layers 1, 3 and 5 can be expressed as Fig. 3 Laminate with two interleaved viscoelastic layer.
5 Passive Damping Characteristics of Carbon Epoxy Composite Plates 39 Plate Clamped at One End and Free at the Other 3. Plate Boundary Condition In the case of a beam clamped at the end x = 0 and free at the other end x = L, its geometric representation is shown in Fig. 4 and the boundary conditions are At the end x = 0: Fig. 4 Clamped Free Beam condition. U ort pq = U 1 pq + U 3 pq + U 5 pq = ort A mn A ij f pq (θ)d pq m=1 n=1 i=1 j=1 pq = 11,12,22,66 With, D ort pq = e 0 e 3 + α α 2 3 α e 0 e 3 (10) (11) α e 3 0 e e 3 Qpq 24 The strain energy stored in the two viscoelastic layers 2 and 4 can be written as U v pq = 1 2Ra 2 A mna ij f v v pq (θ v )D pq With, m=1 n=1 i=1 j=1 D v pq = α e 0 e 3 + α e 0 e 3 e3 (12) (13) (α 1 + α 2 ) 3 v iq pq 24 where, the functions f v pq (θ v ) are given by Eq. (5). In the particular case of two viscoelastic layers which are interleaved at the same distance from the middle plane d 1 = d 2 = α e (14) 2 Hence the bending stiffness induced by the viscoelastic layers are simply written as D v pq = α + 2 e 3 0 e (α) 3 v iq e3 (15) pq 12 w 0 (x = 0) = 0, dw 0 dx (x = 0) = 0 (16) At the end x = L: w 0 (x = L) = 0, (x = L) = 0, (17) Also, d 2 w 0 dx 2 (x = L) = 0, d3 w 0 dx 3 (x = L) = 0, (18) The first eight solutions of Equation for clamped free beam are listed in Table 1 with the corresponding values of γ m. For high enough values of γ m the approximate values can be written in the form λ m = (m )π (19) In the case of a beam that is free at both ends its geometric representation is shown in figure. 5 and the boundary conditions are: d 2 X m dx 2 d 2 X m dx 2 With, (x = 0) = 0, d3 X m (x = 0) = 0, dx3 (x = L) = 0, d3 X m (x = L) = 0, dx3 X 1 (x) = 1, (20) X 2 (x) = 2 3 x L 1 (21) These functions correspond to the rigid modes of translation and rotation. The two roots λ 1 = 0 and λ 2 = 0 are associated with these functions. The other roots λ m and the corresponding values γ m are identical to those found in the case of two clamped ends. The values of λ m and γ m are given in Table 2 for m varying from 1 to 9. The first mode of free vibrations is obtained for m = 3. The free vibration frequencies are identical to those of a beam with clamped ends. 4. aterials Selection Each of the composite plates was chosen to have the following physical and geometric configuration:
6 40 Passive Damping Characteristics of Carbon Epoxy Composite Plates Table 1 Coefficients of a clampedfree beam function. m λ m γ m ((m0.5)π Plate with two free ends Fig. 5 Free Free Beam condition. Length (a) = 300 mm Breadth (b) = 200 mm o of plies (n) = 8 Thickness of each ply (t) = 0.3 mm Force (q 0 ) = 500 Thickness of Viscoelastic material (e 0 ) = 0.2 mm The materials properties of chosen materials listed in Table Results and Discussion Loss factor (η) of unidirectional carbon fibre/epoxy laminate with different boundary conditions and at various fibre orientations for a single and multiple viscoelastic layer positions from the laminate mid plane. Case I: (CFFF) One edge clamped all other edges free. Case II: (CCCC) All edges clamped. Case III: (CFCF) Adjacent edges clamped. The loss factor (η) of Unidirectional Carbon Fibres/Epoxy with different boundary conditions and at various fibre orientations without and with Viscoelastic Layers is shown in Table 4. and Table 5 respevtively. Figs 6 and 7 are the plot of results displayed in Tables 4 and 5 i.e loss factor as a function of fiber orientation. Table 2 Coefficients of a freefree beam function. m λ m γ m Table 3 aterials properties of glass/epoxy and viscoelastic layer. aterial E L (GPa) E T (GPa) G LT (GPa) υ LT η 11 (%) η 22 (%) η 66 (%) Carbon/Epoxy Viscoelastic 50 (Pa) 50 (Pa) 50 (pa) Table 4 Loss factor (η) of unidirectional carbon fibres/epoxy with different boundary conditions and at various fibre orientations without viscoelastic layers. Angle CCCC CFFF CFCF
7 Passive Damping Characteristics of Carbon Epoxy Composite Plates 41 Table 5 Loss factor (η) of unidirectional carbon fibres/epoxy with CFCF boundary conditions and at various fibre orientations with viscoelastic layers. Angle Loss factor (η) of carbon/ epoxy laminate CFCF id Sym Asym Outer Loss Factor Fibre Orientation Fig. 6 Variation of Loss factor (η) of unidirectional carbon fibres with fibre orientation without viscoelastic layers. Loss Factor CCCC CFFF CFCF idplane 0.6 Symm Asymm Outer Fibre Orientation Fig. 7 Loss factor (η) of unidirectional carbon fibres (CFCF) with viscoelastic material inserted at various positions with fibre orientation. 6. Conclusions This study investigates the damping properties of unidirectional carbon reinforced laminates shows very poor damping values when compared with glass and Kevlar reinforced laminates [3]. But, when it is provided with interleaved constrain layer with a single or two its damping values obtain are considerably high. For a given laminate without constrain layer, the CFCF (Fig. 6) will have maximum value of loss factor at Whereas the minimum value for the same boundary conditions recorded at 15 0 if a constrain layer is used at midplane position. For all other positions of constrain layer the loss factor is in between 0.5% at 30 0 single midplane to 1.97% at 90 0 two outer position. It shows that damping nature of carbon laminates and 90 0 enhanced four folds. It is also realized that the provision of constrain layer in the FRP lamination process is highly compatible. It is noticed that a trend of increase in the damping of laminates significant as the viscoelastic layers are placed from the mid layer to outer layer. Also it showed that, the least value of loss factor found at 30 0 when two layers are used irrespective of their locations. References [1] Adams, R. D. and aheri,. R Dynamic Flexural Properties of Anisotropic FIbrous Composite Beams. Compos Sci Technol 50 (4): [2] Billups, E. K. and Cavalli, DDamping Predictions of Fibre Composite Plates: Layup Effects. Compos. Sci. Technol. 68 :
8 42 Passive Damping Characteristics of Carbon Epoxy Composite Plates [3] aheri, A.., Assarar,., Sefrani, Y. and Berthelot, J Damping Analysis of Orthotropic Composite aterials and Laminates Composites. 39: [4] Berthelot, J.. and Sefrani, Y Damping Analysis of Unidirectional Glass and Kevlar Fibre Composites. Composites Science and Technology 64: [5] Li, J.Q. and arita, Y Analysis and Optimal Design for the Damping Property of Laminated Viscoelastic Plates under General Edge Conditions. Composites: Part B 45: [6] Berthelot, J Damping Analysis of Orthotropic Composites with Interleaved Viscoelastic Layers: odelling. Journal of Composite aterials 40 (21): [7] i, R. G. and Adams, R. D The Damping and Dynamic oduli of Symmetric Laminated Composite BeamsTheoretical and Experimental Results. J. Compos ater 18 (2):
Passive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationVIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS
Journal of Engineering Science and Technology Vol. 12, No. 12 (217) 33983411 School of Engineering, Taylor s University VIBRATION CONTROL OF RECTANGULAR CROSSPLY FRP PLATES USING PZT MATERIALS DILEEP
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationDynamic Response Of Laminated Composite Shells Subjected To Impulsive Loads
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 14, Issue 3 Ver. I (May.  June. 2017), PP 108123 www.iosrjournals.org Dynamic Response Of Laminated
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More informationDynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load
Dynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationSTUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES
Int. J. of Applied Mechanics and Engineering, 214, vol.19, No.1, pp.2329 DOI: 1.2478/ijame21415 Brief note STUDY OF THE EFFECT OF COMPOSITE CONSTRAINED LAYERS IN VIBRATION DAMPING OF PLATES K.S.K. SASIKUMAR
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. B. (2015) Influence of bending twisting coupling on compression and shear buckling strength. Stability of Structures 14th Symposium, Zakopane, Poland, 812 Jun 2015. Copyright 2015 The Author.
More informationI INTRODUCTION II THEORY
Estimation of Loss Factor of Viscoelastic Material by Using Cantilever Sandwich Plate 1 Jitender Kumar, 2 Dr. Rajesh Kumar 1 Geeta Engineering College (Panipat) 2 SLIET Longowal, Punjab 1 jitd2007@rediffmail.com
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationEffect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure
IOP Conference Series: Materials Science and Engineering PAPER OPEN ACCESS Effect of magnetostrictive material layer on the stress and deformation behaviour of laminated structure To cite this article:
More informationA Numerical Study on Prediction of BFS in Composite Structures under Ballistic Impact
VOL. 1, 2015 ISSN 2394 3750 EISSN 2394 3769 SCIENCE & TECHNOLOGY A Numerical Study on Prediction of BFS in Composite Structures under Ballistic Impact Bandaru Aswani Kumar 1, Suhail Ahmad 2 1. Research
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationMaterial Characterization of Carbon Fiber Reinforced Polymer Laminate Using Virtual Fields Method
Proceedings of ICTACEM 014 International Conference on Theoretical, Applied, Computational and Experimental Mechanics December 931, 014, IIT Kharagpur, India ICTACEM014/39 Material Characterization of
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationFinite element analysis of FRP pipelines dynamic stability
Boundary Elements and Other esh Reduction ethods XXXVIII 39 Finite element analysis of FRP pipelines dynamic stability D. G. Pavlou & A. I. Nergaard Department of echanical and Structural Engineering and
More informationDesign of Hybrid Composites for Axial loads with Zero Coefficient of Thermal Expansion
Design of Hybrid Composites for Axial loads with Zero Coefficient of Thermal Expansion Zaffar M. Khan 1 and Asim Shahzad 2 Institute of Space Technology, Islamabad, Pakistan, 44000 Aerospace structures
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationDEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL
DEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL S. Quinn*, R.K. Fruehmann and J.M. DulieuBarton School of Engineering Sciences University of Southampton Southampton SO17
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationAnalysis of Flexural Properties of Carbon Fiber Reinforced / EPoxy Composite Material
ISSN 23951621 Analysis of Flexural Properties of Carbon Fiber Reinforced / EPoxy Composite Material #1 Kishor Shingare, #2 Dr. S.M. Shendokar, #3 Prof. P.V. Deshmukh, #4 Prof. S.S. Chavan 1 kishorshingare911@gmail.com
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationVibration Modelling of Composite Laminates with Delamination Damage
Proceedings of 20 th International Congress on Acoustics, ICA 2010 2327 August 2010, Sydney, Australia Vibration Modelling of Composite Laminates with Delamination Damage Z. Zhang, K. Shankar, M. Tahtali
More informationThermal Vibration of Magnetostrictive Material in Laminated Plates by the GDQ Method
The Open echanics Journal, 007, 1, 937 9 Thermal Vibration of agnetostrictive aterial in Laminated Plates by the GDQ ethod C.C. Hong * Department of echanical Engineering, Hsiuping Institute of Technology,
More informationTheoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates
*Manuscript Click here to view linked References 1 1 1 1 1 1 1 0 1 0 1 0 1 0 1 0 1 Theoretical Approach to Predict Transverse Impact Response of VariableStiffness Curved Composite Plates B. Arachchige,
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationInfluence of Inherent Material Damping on the Dynamic Buckling of Composite Columns with Open Cross Sections
Mechanics and Mechanical Engineering Vol. 17, No. 1 (2013) 59 69 c Lodz University of Technology Influence of Inherent Material Damping on the Dynamic Buckling of Composite Columns with Open Cross Sections
More informationThermal buckling and postbuckling of laminated composite plates with. temperature dependent properties by an asymptotic numerical method
hermal buckling and postbuckling of laminated composite plates with temperature dependent properties by an asymptotic numerical method F. Abdoun a,*, L. Azrar a,b, E.M. Daya c a LAMA, Higher School of
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationComposite Materials Research Laboratory, State University of New York at Buffalo, Buffalo, NY , USA
Composite Interfaces, Vol. 7, No. 4, pp. 257 275 (2000) VSP 2000. Discontinuous surfacetreated submicrondiameter carbon filaments as an interlaminar filler in carbon fiber polymermatrix composites for
More informationINTERNAL STRAIN MEASUREMENTS IN CFRP PLATES SUBJECTED TO IMPACT LOAD USING FBG SENSORS
INTERNAL STRAIN MEASUREMENTS IN CFRP PLATES SUBJECTED TO IMPACT LOAD USING FBG SENSORS J. Frieden, J. Cugnoni, J. Botsis, Th. Gmür, D. Coric Laboratoire de Mécanique appliquée et d Analyse de Fiabilité
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More informationThe Rotating Inhomogeneous Elastic Cylinders of. VariableThickness and Density
Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of VariableThickness and
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationComposite Structural Mechanics using MATLAB
Session 2520 Composite Structural Mechanics using MATLAB Oscar Barton, Jr., Jacob B. Wallace United States Naval Academy Annapolis, Md 21402 Abstract In this paper MATLAB is adopted as the programming
More informationBENDING VIBRATIONS OF ROTATING NONUNIFORM COMPOSITE TIMOSHENKO BEAMS WITH AN ELASTICALLY RESTRAINED ROOT
BENDING VIBRATIONS OF ROTATING NONUNIFORM COMPOSITE TIMOSHENKO BEAMS WITH AN EASTICAY RESTRAINED ROOT Sen Yung ee and Jin Tang Yang Department of Mechanical Engineering, National Cheng Kung University,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationOPTIMAL FIBER PLACEMENT INCLUDING EFFECTS OF EMBROIDERY
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL FIBER PLACEMENT INCLUDING EFFECTS OF EMBROIDERY T. Nishida 1 T. Ieda 2 * A. Senba 2 1 Department of Aerospace Engineering Nagoya University
More informationIDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationFor an imposed stress history consisting of a rapidly applied stepfunction jump in
Problem 2 (20 points) MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING CAMBRIDGE, MASSACHUSETTS 0239 2.002 MECHANICS AND MATERIALS II SOLUTION for QUIZ NO. October 5, 2003 For
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationFree Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires
11(2014) 279298 Free Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires Abstract In this paper, free vibration response of a hybrid composite plate was studied. Effects
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationAnalysis and Optimization of a Hybrid Fan Blade
Analysis and Optimization of a Hybrid Fan Blade Permas Users Conference 27.04.06 28.04.06 Strassbourg DLR German Aerospace Center, Stuttgart Institute of Structures and Design J. Ehrmanntraut, F. Kocian,
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationCOMPARISON OF PLATE MODELS FOR ANALYSIS OF LAMINATED COMPOSITES
COMPARISON OF PLATE MODELS FOR ANALYSIS OF LAMINATED COMPOSITES P. M. Mohite and C. S. Upadhyay** Department of Aerospace Engineering, IIT Kanpur 0806, INDIA, email: mohite@iitk.ac.in Assistant Professor,
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More information